Presentation on theme: "Chapter 14 - 1 ISSUES TO ADDRESS... What are the general structural and chemical characteristics of polymer molecules? What are some of the common polymeric."— Presentation transcript:
Chapter 14 - 1 ISSUES TO ADDRESS... What are the general structural and chemical characteristics of polymer molecules? What are some of the common polymeric materials, and how do they differ chemically? How is the crystalline state in polymers different from that in metals and ceramics ? Chapter 14: Polymer Structures
Chapter 14 - 2 What is a Polymer? Poly mer many repeat unit Adapted from Fig. 14.2, Callister & Rethwisch 8e. CCCCCC HHHHHH HHHHHH Polyethylene (PE) Cl CCCCCC HHH HHHHHH Poly(vinyl chloride) (PVC) HH HHHH Polypropylene (PP) CCCCCC CH 3 HH H repeat unit repeat unit repeat unit
Chapter 14 - 3 Ancient Polymers Originally natural polymers were used –Wood– Rubber –Cotton– Wool –Leather– Silk Oldest known uses –Rubber balls used by Incas –Noah used pitch (a natural polymer) for the ark
Chapter 14 - 4 Polymer Composition Most polymers are hydrocarbons – i.e., made up of H and C Saturated hydrocarbons –Each carbon singly bonded to four other atoms –Example: Ethane, C 2 H 6
6 Unsaturated Hydrocarbons Double & triple bonds somewhat unstable – can form new bonds –Double bond found in ethylene or ethene - C 2 H 4 –Triple bond found in acetylene or ethyne - C 2 H 2
Chapter 14 - 7 Isomerism –two compounds with same chemical formula can have quite different structures for example: C 8 H 18 normal-octane 2,4-dimethylhexane
Chapter 14 - 8 Polymerization and Polymer Chemistry Free radical polymerization Initiator: example - benzoyl peroxide
Chapter 14 - 9 Chemistry and Structure of Polyethylene Adapted from Fig. 14.1, Callister & Rethwisch 8e. Note: polyethylene is a long-chain hydrocarbon - paraffin wax for candles is short polyethylene
Chapter 14 - 11 Bulk or Commodity Polymers (cont)
Chapter 14 - 12 Bulk or Commodity Polymers (cont)
Chapter 14 - VMSE: Polymer Repeat Unit Structures 13 Manipulate and rotate polymer structures in 3-dimensions
Chapter 14 - 14 MOLECULAR WEIGHT Molecular weight, M: Mass of a mole of chains. Low M high M Not all chains in a polymer are of the same length — i.e., there is a distribution of molecular weights
Chapter 14 - 15 x i = number fraction of chains in size range i MOLECULAR WEIGHT DISTRIBUTION Adapted from Fig. 14.4, Callister & Rethwisch 8e. w i = weight fraction of chains in size range i M i = mean (middle) molecular weight of size range i
Chapter 14 - 16 Molecular Weight Calculation Example: average mass of a class StudentWeight mass (lb) 1104 2116 3140 4143 5180 6182 7191 8220 9225 10380 What is the average weight of the students in this class: a)Based on the number fraction of students in each mass range? b)Based on the weight fraction of students in each mass range?
Chapter 14 - 17 Molecular Weight Calculation (cont.) Solution: The first step is to sort the students into weight ranges. Using 40 lb ranges gives the following table: total number total weight Calculate the number and weight fraction of students in each weight range as follows: For example: for the 81-120 lb range
Chapter 14 - 19 Degree of Polymerization, DP DP = average number of repeat units per chain DP = 6 mol. wt of repeat unit iChain fraction
Chapter 14 - 20 Adapted from Fig. 14.7, Callister & Rethwisch 8e. Molecular Structures for Polymers BranchedCross-LinkedNetworkLinear secondary bonding
Chapter 14 - 21 Polymers – Molecular Shape Molecular Shape (or Conformation) – chain bending and twisting are possible by rotation of carbon atoms around their chain bonds –note: not necessary to break chain bonds to alter molecular shape Adapted from Fig. 14.5, Callister & Rethwisch 8e.
Chapter 14 - 22 Chain End-to-End Distance, r Adapted from Fig. 14.6, Callister & Rethwisch 8e.
Chapter 14 - 23 Molecular Configurations for Polymers Configurations – to change must break bonds Stereoisomerism E B A D CC D A B E mirror plane Stereoisomers are mirror images – can’t superimpose without breaking a bond
Chapter 14 - 24 Tacticity Tacticity – stereoregularity or spatial arrangement of R units along chain isotactic – all R groups on same side of chain syndiotactic – R groups alternate sides
Chapter 14 - 25 Tacticity (cont.) atactic – R groups randomly positioned
Chapter 14 - 26 cis/trans Isomerism cis cis-isoprene (natural rubber) H atom and CH 3 group on same side of chain trans trans-isoprene (gutta percha) H atom and CH 3 group on opposite sides of chain
Chapter 14 - VMSE: Stereo and Geometrical Isomers 27 Chapter 7 - 19 Manipulate and rotate polymer structures in 3-dimensions
Chapter 14 - 28 Copolymers two or more monomers polymerized together random – A and B randomly positioned along chain alternating – A and B alternate in polymer chain block – large blocks of A units alternate with large blocks of B units graft – chains of B units grafted onto A backbone A – B – random block graft Adapted from Fig. 14.9, Callister & Rethwisch 8e. alternating
Chapter 14 - 29 Crystallinity in Polymers Ordered atomic arrangements involving molecular chains Crystal structures in terms of unit cells Example shown –polyethylene unit cell Adapted from Fig. 14.10, Callister & Rethwisch 8e.
Chapter 14 - 30 Polymer Crystallinity Crystalline regions –thin platelets with chain folds at faces –Chain folded structure 10 nm Adapted from Fig. 14.12, Callister & Rethwisch 8e.
Chapter 14 - 31 Polymer Crystallinity (cont.) Polymers rarely 100% crystalline Difficult for all regions of all chains to become aligned Degree of crystallinity expressed as % crystallinity. -- Some physical properties depend on % crystallinity. -- Heat treating causes crystalline regions to grow and % crystallinity to increase. Adapted from Fig. 14.11, Callister 6e. (Fig. 14.11 is from H.W. Hayden, W.G. Moffatt, and J. Wulff, The Structure and Properties of Materials, Vol. III, Mechanical Behavior, John Wiley and Sons, Inc., 1965.) crystalline region amorphous region
Chapter 14 - 32 Polymer Single Crystals Electron micrograph – multilayered single crystals (chain-folded layers) of polyethylene Single crystals – only for slow and carefully controlled growth rates Adapted from Fig. 14.11, Callister & Rethwisch 8e.
Chapter 14 - 33 Semicrystalline Polymers Spherulite surface Adapted from Fig. 14.13, Callister & Rethwisch 8e. Some semicrystalline polymers form spherulite structures Alternating chain-folded crystallites and amorphous regions Spherulite structure for relatively rapid growth rates
Chapter 14 - 34 Photomicrograph – Spherulites in Polyethylene Adapted from Fig. 14.14, Callister & Rethwisch 8e. Cross-polarized light used -- a maltese cross appears in each spherulite